Download presentation

Presentation is loading. Please wait.

Published byCourtney Hailes Modified over 2 years ago

1
Estimating Crystallite Size Using XRD Scott A Speakman, Ph.D. 13-4009A speakman@mit.edu http://prism.mit.edu/xray MIT Center for Materials Science and Engineering

2
Center for Materials Science and Engineering http://prism.mit.edu/xray Warning These slides have not been extensively proof-read, and therefore may contain errors. While I have tried to cite all references, I may have missed some– these slides were prepared for an informal lecture and not for publication. If you note a mistake or a missing citation, please let me know and I will correct it. I hope to add commentary in the notes section of these slides, offering additional details. However, these notes are incomplete so far.

3
Center for Materials Science and Engineering http://prism.mit.edu/xray Goals of Today’s Lecture Provide a quick overview of the theory behind peak profile analysis Discuss practical considerations for analysis Briefly mention other peak profile analysis methods –Warren Averbach Variance method –Mixed peak profiling –whole pattern Discuss other ways to evaluate crystallite size Assumptions: you understand the basics of crystallography, X-ray diffraction, and the operation of a Bragg-Brentano diffractometer

4
Center for Materials Science and Engineering http://prism.mit.edu/xray A Brief History of XRD 1895- Röntgen publishes the discovery of X-rays 1912- Laue observes diffraction of X-rays from a crystal 1913- Bragg solves the first crystal structure from X-ray diffraction data when did Scherrer use X-rays to estimate the crystallite size of nanophase materials?when did Scherrer use X-rays to estimate the crystallite size of nanophase materials?

5
Center for Materials Science and Engineering http://prism.mit.edu/xray The Scherrer Equation was published in 1918 Peak width (B) is inversely proportional to crystallite size (L) P. Scherrer, “Bestimmung der Grösse und der inneren Struktur von Kolloidteilchen mittels Röntgenstrahlen,” Nachr. Ges. Wiss. Göttingen 26 (1918) pp 98-100. J.I. Langford and A.J.C. Wilson, “Scherrer after Sixty Years: A Survey and Some New Results in the Determination of Crystallite Size,” J. Appl. Cryst. 11 (1978) pp 102-113.

6
Center for Materials Science and Engineering X-Ray Peak Broadening is caused by deviation from the ideal crystalline lattice The Laue Equations describe the intensity of a diffracted peak from an ideal parallelopipeden crystal The ideal crystal is an infinitely large and perfectly ordered crystalline array –From the perspective of X-rays, “infinitely” large is a few microns Deviations from the ideal create peak broadening –A nanocrystallite is not “infinitely” large –Non-perfect ordering of the crystalline array can include Defects Non-uniform interplanar spacing disorder http://prism.mit.edu/xray

7
Center for Materials Science and Engineering http://prism.mit.edu/xray As predicted by the Laue equations, the diffraction peaks becomes broader when N is not infinite N 1, N 2, and N 3 are the number of unit cells along the a 1, a 2, and a 3 directions The calculated peak is narrow when N is a large number (ie infinitely large) When N is small, the diffraction peaks become broader –A nanocrystalline phase has a small number of N The peak area remains constant independent of N

8
Center for Materials Science and Engineering 666768697071727374 2 (deg.) Intensity (a.u.) http://prism.mit.edu/xray We cannot assume that all broad peaks are produced by nanocrystalline materials These diffraction patterns were produced from the exact same sample Two different diffractometers, with different optical configurations, were used The apparent peak broadening is due solely to the instrumentation

9
Center for Materials Science and Engineering http://prism.mit.edu/xray Many factors may contribute to the observed peak profile Instrumental Peak Profile Crystallite Size Microstrain –Non-uniform Lattice Distortions –Faulting –Dislocations –Antiphase Domain Boundaries –Grain Surface Relaxation Solid Solution Inhomogeneity Temperature Factors The peak profile is a convolution of the profiles from all of these contributionsThe peak profile is a convolution of the profiles from all of these contributions

10
Center for Materials Science and Engineering 46.746.846.947.047.147.247.347.447.547.647.747.847.9 2 (deg.) Intensity (a.u.) http://prism.mit.edu/xray 46.746.846.947.047.147.247.347.447.547.647.747.847.9 2 (deg.) Intensity (a.u.) Before analysis, you must decide how you will define Peak Width Full Width at Half Maximum (FWHM) –the width of the diffraction peak, in radians, at a height half-way between background and the peak maximum –This was most often used in older research because it is easier to calculate Integral Breadth –the total area under the peak divided by the peak height –the width of a rectangle having the same area and the same height as the peak –requires very careful evaluation of the tails of the peak and the background FWHM

11
Center for Materials Science and Engineering http://prism.mit.edu/xray Integral Breadth may be the way to define peak width with modern analysis software Warren suggests that the Stokes and Wilson method of using integral breadths gives an evaluation that is independent of the distribution in size and shape –L is a volume average of the crystal thickness in the direction normal to the reflecting planes –The Scherrer constant K can be assumed to be 1 Langford and Wilson suggest that even when using the integral breadth, there is a Scherrer constant K that varies with the shape of the crystallites

12
Center for Materials Science and Engineering http://prism.mit.edu/xray Other methods used to determine peak width These methods are used in more the variance methods, such as Warren-Averbach analysis –Most often used for dislocation and defect density analysis of metals –Can also be used to determine the crystallite size distribution –Requires no overlap between neighboring diffraction peaks Variance-slope –the slope of the variance of the line profile as a function of the range of integration Variance-intercept –negative initial slope of the Fourier transform of the normalized line profile

13
Center for Materials Science and Engineering http://prism.mit.edu/xray Instrument and Sample Contributions to the Peak Profile must be Deconvoluted In order to analyze crystallite size, we must deconvolute: –Instrumental Broadening FW(I) also referred to as the Instrumental Profile, Instrumental FWHM Curve, Instrumental Peak Profile –Specimen Broadening FW(S) also referred to as the Sample Profile, Specimen Profile We must then separate the different contributions to specimen broadening –Crystallite size and microstrain broadening of diffraction peaks This requires an Instrument Profile Calibration Curve

14
Center for Materials Science and Engineering 47.047.247.447.647.8 2 (deg.) Intensity (a.u.) http://prism.mit.edu/xray The Instrument Peak Profile Calibration Curve quantifies the contribution of the instrument to the observed peak widths The peak widths from the instrument peak profile are a convolution of: –X-ray Source Profile Wavelength widths of K 1 and K 2 lines Size of the X-ray source Superposition of K 1 and K 2 peaks –Goniometer Optics Divergence and Receiving Slit widths Imperfect focusing Beam size Penetration into the sample Patterns collected from the same sample with different instruments and configurations at MIT

15
Center for Materials Science and Engineering http://prism.mit.edu/xray Other Instrumental and Sample Considerations for Thin Films The irradiated area greatly affects the intensity of high angle diffraction peaks –GIXD or variable divergence slits on the PANalytical X’Pert Pro will maintain a constant irradiated area, increasing the signal for high angle diffraction peaks –both methods increase the instrumental FWHM Bragg-Brentano geometry only probes crystallite dimensions through the thickness of the film –in order to probe lateral (in-plane) crystallite sizes, need to collect diffraction patterns at different tilts –this requires the use of parallel-beam optics on the PANalytical X’Pert Pro, which have very large FWHM and poor signal:noise ratios

16
Center for Materials Science and Engineering http://prism.mit.edu/xray In order to build a Instrument Peak Profile Calibration Curve Collect data from a standard using the exact instrument and configuration as will be used for analyzing the sample –same optical configuration of diffractometer –same sample preparation geometry –You need a separate calibration curve for every different instrument and instrument configuration Even a small change, such as changing the divergence slit from ½ to ¼° aperture, will change the instrument profile –calibration curve should cover the 2theta range of interest for the specimen diffraction pattern do not extrapolate the calibration curve Profile fit the diffraction peaks from the standard Fit the peak widths to a function such as the Cagliotti equation. Use this function as the calibration curve.

17
Center for Materials Science and Engineering The Cagliotti equation describes how peak width varies with 2theta H k is the Cagliotti function where U, V and W are refinable parameters

18
Center for Materials Science and Engineering http://prism.mit.edu/xray Selecting a standard for building the Instrument Peak Profile Calibration Curve Standard should share characteristics with the nanocrystalline specimen –Similar linear absorption coefficient similar mass absorption coefficient similar atomic weight similar packing density The standard should not contribute to the diffraction peak profile –macrocrystalline: crystallite size larger than 500 nm –particle size less than 10 microns –defect and strain free There are several calibration techniques –Internal Standard –External Standard of same composition –External Standard of different composition

19
Center for Materials Science and Engineering http://prism.mit.edu/xray Internal Standard Method for Calibration Mix a standard in with your nanocrystalline specimen a NIST certified standard is preferred –use a standard with similar mass absorption coefficient –NIST 640c Si –NIST 660a LaB 6 –NIST 674b CeO 2 –NIST 675 Mica standard should have few, and preferably no, overlapping peaks with the specimen –overlapping peaks will greatly compromise accuracy of analysis

20
Center for Materials Science and Engineering http://prism.mit.edu/xray Internal Standard Method for Calibration Advantages: –know that standard and specimen patterns were collected under identical circumstances for both instrumental conditions and sample preparation conditions –the linear absorption coefficient of the mixture is the same for standard and specimen Disadvantages: –difficult to avoid overlapping peaks between standard and broadened peaks from very nanocrystalline materials –the specimen becomes contaminated –only works with a powder specimen

21
Center for Materials Science and Engineering http://prism.mit.edu/xray External Standard Method for Calibration If internal calibration is not an option, then use external calibration Run calibration standard separately from specimen, keeping as many parameters identical as is possible The best external standard is a macrocrystalline specimen of the same phase as your nanocrystalline specimen –How can you be sure that macrocrystalline specimen does not contribute to peak broadening?

22
Center for Materials Science and Engineering http://prism.mit.edu/xray Qualifying your Macrocrystalline Standard select powder for your potential macrocrystalline standard –if not already done, possibly anneal it to allow crystallites to grow and to allow defects to heal use internal calibration to validate that macrocrystalline specimen is an appropriate standard –mix macrocrystalline standard with appropriate NIST SRM –compare FWHM curves for macrocrystalline specimen and NIST standard –if the macrocrystalline FWHM curve is similar to that from the NIST standard, than the macrocrystalline specimen is suitable –collect the XRD pattern from pure sample of you macrocrystalline specimen do not use the FHWM curve from the mixture with the NIST SRM

23
Center for Materials Science and Engineering http://prism.mit.edu/xray Disadvantages/Advantages of External Calibration with a Standard of the Same Composition Advantages: –will produce better calibration curve because mass absorption coefficient, density, molecular weight are the same as your specimen of interest –can duplicate a mixture in your nanocrystalline specimen –might be able to make a macrocrystalline standard for thin film samples Disadvantages: –time consuming –desire a different calibration standard for every different nanocrystalline phase and mixture –macrocrystalline standard may be hard/impossible to produce –calibration curve will not compensate for discrepancies in instrumental conditions or sample preparation conditions between the standard and the specimen

24
Center for Materials Science and Engineering http://prism.mit.edu/xray External Standard Method of Calibration using a NIST standard As a last resort, use an external standard of a composition that is different than your nanocrystalline specimen –This is actually the most common method used –Also the least accurate method Use a certified NIST standard to produce instrumental FWHM calibration curve –Use the standard that has the most similar linear absorption coefficient

25
Center for Materials Science and Engineering http://prism.mit.edu/xray Advantages and Disadvantages of using NIST standard for External Calibration Advantages –only need to build one calibration curve for each instrumental configuration –I have NIST standard diffraction patterns for each instrument and configuration available for download from http://prism.mit.edu/xray/standards.htm –know that the standard is high quality if from NIST –neither standard nor specimen are contaminated Disadvantages –The standard may behave significantly different in diffractometer than your specimen different mass absorption coefficient different depth of penetration of X-rays –NIST standards are expensive –cannot duplicate exact conditions for thin films

26
Center for Materials Science and Engineering http://prism.mit.edu/xray Consider- when is good calibration most essential? For a very small crystallite size, the specimen broadening dominates over instrumental broadening Only need the most exacting calibration when the specimen broadening is small because the specimen is not highly nanocrystalline FWHM of Instrumental Profile at 48° 2 0.061 deg Broadening Due to Nanocrystalline Size Crystallite Size B(2 ) (rad) FWHM (deg) 100 nm0.00150.099 50 nm0.00290.182 10 nm0.01450.871 5 nm0.02911.745

27
Center for Materials Science and Engineering http://prism.mit.edu/xray What Instrument to Use? The instrumental profile determines the upper limit of crystallite size that can be evaluated –if the Instrumental peak width is much larger than the broadening due to crystallite size, then we cannot accurately determine crystallite size –For analyzing larger nanocrystallites, it is important to use the instrument with the smallest instrumental peak width Very small nanocrystallites produce weak signals –the specimen broadening will be significantly larger than the instrumental broadening –the signal:noise ratio is more important than the instrumental profile

28
Center for Materials Science and Engineering http://prism.mit.edu/xray Comparison of Peak Widths at 47 ° 2 for Instruments and Crystallite Sizes Instruments with better peak height to background ratios are better for small nanocrystallites, <20nm Instruments with smaller instrumental peak widths are better for larger nanocrystallites, >80 nm ConfigurationFWHM (deg) Pk Ht to Bkg Ratio 185mm radius, 0.5° DS, diffracted-beam monochromator, point detector 0.124339 240mm radius, 0.25° DS, beta-filter, linear PSD 0.06081 240mm radius, 0.5° DS, beta-filter, linear PSD 0.07772 240mm radius, 0.5° DS, diffracted-beam monochromator, linear PSD 0.073111 Gobel mirror, 0.09° Parallel Beam Collimator0.17550 Gobel mirror, 0.27° Parallel Beam Collimator0.19455 Crystallite Size FWHM (deg) 100 nm0.099 50 nm0.182 10 nm0.871 5 nm1.745

29
Center for Materials Science and Engineering For line profile analysis, must remove the instrument contribution to each peak list http://prism.mit.edu/xray

30
Center for Materials Science and Engineering http://prism.mit.edu/xray Once the instrument broadening contribution has been remove, the specimen broadening can be analyzed Contributions to specimen broadening –Crystallite Size –Microstrain Non-uniform Lattice Distortions Faulting Dislocations Antiphase Domain Boundaries Grain Surface Relaxation –Solid Solution Inhomogeneity –Temperature Factors The peak profile is a convolution of the profiles from all of these contributionsThe peak profile is a convolution of the profiles from all of these contributions

31
Center for Materials Science and Engineering http://prism.mit.edu/xray Crystallite Size Broadening Peak Width due to crystallite size varies inversely with crystallite size –as the crystallite size gets smaller, the peak gets broader The peak width varies with 2 as cos –The crystallite size broadening is most pronounced at large angles 2Theta However, the instrumental profile width and microstrain broadening are also largest at large angles 2theta peak intensity is usually weakest at larger angles 2theta –If using a single peak, often get better results from using diffraction peaks between 30 and 50 deg 2theta below 30deg 2theta, peak asymmetry compromises profile analysis

32
Center for Materials Science and Engineering http://prism.mit.edu/xray The Scherrer Constant, K The constant of proportionality, K (the Scherrer constant) depends on the how the width is determined, the shape of the crystal, and the size distribution –K actually varies from 0.62 to 2.08 –the most common values for K are: 0.94 for FWHM of spherical crystals with cubic symmetry 0.89 for integral breadth of spherical crystals w/ cubic symmetry 1, because 0.94 and 0.89 both round up to 1 For an excellent discussion of K, refer to JI Langford and AJC Wilson, “Scherrer after sixty years: A survey and some new results in the determination of crystallite size,” J. Appl. Cryst. 11 (1978) p102-113.

33
Center for Materials Science and Engineering http://prism.mit.edu/xray Factors that affect K and crystallite size analysis how the peak width is defined –Whether using FWHM or Integral Breadth Integral breadth is preferred how crystallite size is defined the shape of the crystal the size distribution

34
Center for Materials Science and Engineering http://prism.mit.edu/xray How is Crystallite Size Defined Usually taken as the cube root of the volume of a crystallite –assumes that all crystallites have the same size and shape –None of the X-ray diffraction techniques give a crystallite size that exactly matches this definition For a distribution of sizes, the mean size can be defined as –the mean value of the cube roots of the individual crystallite volumes –the cube root of the mean value of the volumes of the individual crystallites Scherrer method (using FWHM) gives the ratio of the root-mean- fourth-power to the root-mean-square value of the thickness Stokes and Wilson method (using integral breadth) determines the volume average of the thickness of the crystallites measured perpendicular to the reflecting plane The variance methods give the ratio of the total volume of the crystallites to the total area of their projection on a plane parallel to the reflecting planes

35
Center for Materials Science and Engineering The Stokes and Wilson method considers that each different diffraction peak is produced from planes along a different crystallographic direction Stokes and Wilson method (using integral breadth) determines the volume average of the thickness of the crystallites measured perpendicular to the reflecting plane This method is useful for identifying anisotropic crystallite shapes http://prism.mit.edu/xray (200) (002) a-axis // [200] c-axis, // [002]

36
Center for Materials Science and Engineering http://prism.mit.edu/xray Remember, Crystallite Size is Different than Particle Size A particle may be made up of several different crystallites Crystallite size often matches grain size, but there are exceptions

37
Center for Materials Science and Engineering The crystallite size observed by XRD is the smallest undistorted region in a crystal Dislocations may create small-angle domain boundaries Dipolar dislocation walls will also create domain boundaries http://prism.mit.edu/xray

38
Center for Materials Science and Engineering http://prism.mit.edu/xray Crystallite Shape Though the shape of crystallites is usually irregular, we can often approximate them as: –sphere, cube, tetrahedra, or octahedra –parallelepipeds such as needles or plates –prisms or cylinders Most applications of Scherrer analysis assume spherical crystallite shapes If we know the average crystallite shape from another analysis, we can select the proper value for the Scherrer constant K Anistropic peak shapes can be identified by anistropic peak broadening –if the dimensions of a crystallite are 2x * 2y * 200z, then (h00) and (0k0) peaks will be more broadened then (00l) peaks.

39
Center for Materials Science and Engineering http://prism.mit.edu/xray Anistropic Size Broadening The broadening of a single diffraction peak is the product of the crystallite dimensions in the direction perpendicular to the planes that produced the diffraction peak.

40
Center for Materials Science and Engineering http://prism.mit.edu/xray Crystallite Size Distribution is the crystallite size narrowly or broadly distributed? is the crystallite size unimodal? XRD is poorly designed to facilitate the analysis of crystallites with a broad or multimodal size distribution Variance methods, such as Warren-Averbach, can be used to quantify a unimodal size distribution –Otherwise, we try to accommodate the size distribution in the Scherrer constant –Using integral breadth instead of FWHM may reduce the effect of crystallite size distribution on the Scherrer constant K and therefore the crystallite size analysis

41
Center for Materials Science and Engineering Values for K referenced in HighScore Plus Values of K from Langford and Wilson, J. Appl. Cryst (1978) are: –0.94 for FWHM of spherical crystals with cubic symmetry –0.89 for integral breadth of spherical crystals w/ cubic symmetry –1, because 0.94 and 0.89 both round up to 1 Assuming the Scherrer definition of crystallite size, values of K listed in the Help for HighScore Plus are: http://prism.mit.edu/xray Crystallite Shape FWHMIntegral Breadth Spheres0.891.07 Cubes0.83 - 0.911.00 – 1.16 Tetrahedra0.73 - 1.030.94 – 1.39 Octahedra0.82 - 0.941.04 – 1.14

42
Center for Materials Science and Engineering Limits for crystallite size analysis There is only broadening due to crystallite size when the crystallite is too small to be considered infinitely large –Above a certain size, there is no peak broadening –The instrument usually constrains the maximum size rather than this limit; this limit only matters for synchrotron and other high resolution instruments The instrument contribution to the peak width may overwhelm the signal from the crystallite size broadening –If the instrument profile is 0.120° with an esd of 0.001°, the maximum resolvable crystallite size will be limited by The precision of the profile fitting, which depends on the peak intensity (weaker peaks give less precise widths) and noise The amount of specimen broadening should be at least 10% of the instrument profile width –In practice, the maximum observed size for a standard laboratory diffractometer is 80 to 120 nm The minimum size requires enough repeating atomic planes to produce the diffraction phenomenon –This depends on the size of the unit cell –The minimum size is typically between 3 to 10 nm, depending on the material http://prism.mit.edu/xray

43
Center for Materials Science and Engineering http://prism.mit.edu/xray Microstrain Broadening lattice strains from displacements of the unit cells about their normal positions often produced by dislocations, domain boundaries, surfaces etc. microstrains are very common in nanoparticle materials the peak broadening due to microstrain will vary as: compare to peak broadening due to crystallite size: Ideal crystal Distorted crystal

44
Center for Materials Science and Engineering http://prism.mit.edu/xray Contributions to Microstrain Broadening Non-uniform Lattice Distortions Dislocations Antiphase Domain Boundaries Grain Surface Relaxation Other contributions to broadening –faulting –solid solution inhomogeneity –temperature factors

45
Center for Materials Science and Engineering http://prism.mit.edu/xray Non-Uniform Lattice Distortions Rather than a single d-spacing, the crystallographic plane has a distribution of d-spaces This produces a broader observed diffraction peak Such distortions can be introduced by: –surface tension of nanoparticles –morphology of crystal shape, such as nanotubes –interstitial impurities 26.527.027.528.028.529.029.530.0 2 (deg.) Intensity (a.u.)

46
Center for Materials Science and Engineering http://prism.mit.edu/xray Antiphase Domain Boundaries Formed during the ordering of a material that goes through an order-disorder transformation The fundamental peaks are not affected the superstructure peaks are broadened –the broadening of superstructure peaks varies with hkl

47
Center for Materials Science and Engineering http://prism.mit.edu/xray Dislocations Line broadening due to dislocations has a strong hkl dependence The profile is Lorentzian Can try to analyze by separating the Lorentzian and Gaussian components of the peak profile Can also determine using the Warren-Averbach method –measure several orders of a peak 001, 002, 003, 004, … 110, 220, 330, 440, … –The Fourier coefficient of the sample broadening will contain an order independent term due to size broadening an order dependent term due to strain

48
Center for Materials Science and Engineering http://prism.mit.edu/xray Faulting Broadening due to deformation faulting and twin faulting will convolute with the particle size Fourier coefficient –The particle size coefficient determined by Warren-Averbach analysis actually contains contributions from the crystallite size and faulting –the fault contribution is hkl dependent, while the size contribution should be hkl independent (assuming isotropic crystallite shape) –the faulting contribution varies as a function of hkl dependent on the crystal structure of the material (fcc vs bcc vs hcp) –See Warren, 1969, for methods to separate the contributions from deformation and twin faulting

49
Center for Materials Science and Engineering http://prism.mit.edu/xray CeO 2 19 nm 4546474849505152 2 (deg.) Intensity (a.u.) ZrO 2 46nm Ce x Zr 1-x O 2 0

50
Center for Materials Science and Engineering http://prism.mit.edu/xray Temperature Factor The Debye-Waller temperature factor describes the oscillation of an atom around its average position in the crystal structure The thermal agitation results in intensity from the peak maxima being redistributed into the peak tails –it does not broaden the FWHM of the diffraction peak, but it does broaden the integral breadth of the diffraction peak The temperature factor increases with 2Theta The temperature factor must be convoluted with the structure factor for each peak –different atoms in the crystal may have different temperature factors –each peak contains a different contribution from the atoms in the crystal

51
Center for Materials Science and Engineering http://prism.mit.edu/xray Scherrer Analysis Calculates Crystallite Size based on each Individual Peak Profile Both crystallite size and microstrain can be calculated based on individual peak profiles IF you assume the other factor is insignificant To test this assumption, look at how the calculated values vary over a long range of 2theta –If the calculated crystallite size or microstrain is consistent over a large range of 2theta, this could indicate that the other factor can be ignored –You cannot make this determination if you use a single diffraction peak –If crystallite size and/or microstrain varies as a function of 2theta, then additional analysis is required. If you have confirmed that crystallite size or microstrain is the only source of specimen broadening for a few samples from a family of specimens, then you MIGHT consider using only single diffraction peak for future analysis.

52
Center for Materials Science and Engineering In this example, crystallite size is consistent over a long range of 2theta Pos. [°2Th.]FWHM Left [°2Th.] Integral Breadth [°2Th.] Crystallite Size only [Å] Micro Strain only [%] Shape Left 28.376(2)1.328(5)2.08665745.5931203.4465141.00(2) 32.929(9)1.52(3)2.38158240.1707203.3828941.00(5) 47.261(5)1.48(1)2.30579043.6862602.1994570.98(2) 56.119(5)1.62(2)2.49278741.8927801.9544950.95(5) 58.85(2)1.6(1)2.39338043.4977001.8021850.9(2) 69.14(1)1.75(5)2.28429448.0025101.4139830.6(3) 76.42(1)1.88(4)2.93494939.8354101.5631261.0(1) 78.80(2)1.96(8)3.07494238.5215201.5751371.0(2) 88.12(1)2.05(7)3.22348339.5981301.3986061.0(3) 95.10(1)2.3(1)3.55086738.2713001.3639081.0(4) Crystallite size varies from 45 to 38 A from 28 to 95 degrees 2theta –The average crystallite size is 4 nm –XRD analysis is only precise to a nm level, not 0.000001 A as the software suggests –In the future, we might use only 1 peak to analyze similar samples http://prism.mit.edu/xray

53
Center for Materials Science and Engineering When both Crystallite Size and Microstrain vary as 2theta, then both are probably present When microstrain is present, the calculated “Crystallite Size only” will tend to decrease as a function of 2theta When crystallite size broadening is present, the calculated “Microstrain only” will tend to decrease as a function of 2theta http://prism.mit.edu/xray Pos. [°2Th.]FWHM Left [°2Th.] Integral Breadth [°2Th.] Crystallite Size only [Å] Micro Strain only [%] Shape Left 40.2733(5)0.829(1)1.30279377.1754301.4496521.000(3) 58.282(2)1.188(5)1.50625469.7112101.1345750.50(1) 73.221(2)1.371(4)2.15426153.5427901.2061821.000(7) 87.053(5)1.67(1)2.51461550.5653801.1059960.91(2) 100.729(5)2.18(2)3.40623842.5669901.1748990.99(2)

54
Center for Materials Science and Engineering A lack of a systematic angular trend for crystallite size or microstrain indicates a more complex complication http://prism.mit.edu/xray Pos. [°2Th.]FWHM Left [°2Th.] Integral Breadth [°2Th.] Crystallite Size only [Å] Micro Strain only [%] Shape Left 21.3278(6)0.143(3)0.224194635.6452000.3274401.00(3) 22.7156(4)0.118(1)0.1648801096.4560000.1783670.74(2) 31.3943(2)0.117(1)0.1687181098.2690000.1296190.81(1) 32.3770(3)0.119(1)0.1705631043.4110000.1323990.79(2) 39.1359(3)0.0990(9)0.1429331739.0080000.0661270.82(1) 43.523(1)0.200(5)0.294495434.8605000.2388960.86(4) 46.4813(4)0.114(1)0.1677961171.4740000.0833190.85(2) 49.674(1)0.179(4)0.272466523.2428000.1752410.93(4) 51.7064(8)0.112(3)0.1764321020.2580000.0865701.00(4) 52.368(1)0.119(3)0.1742151089.1470000.0801400.86(4) 55.3112(8)0.173(3)0.260163563.5067000.1472540.90(2) 57.1989(3)0.108(1)0.1638171429.5350000.0562840.92(1)

55
Center for Materials Science and Engineering http://prism.mit.edu/xray When both crystallite size and microstrain are present, a Williamson-Hall Plot is used y-intercept slope Size broadening Microstrain broadening

56
Center for Materials Science and Engineering http://prism.mit.edu/xray When both crystallite size and microstrain are present, a Williamson-Hall Plot is used y-intercept slope FW(S)*Cos(Theta) Sin(Theta) 0.0000.784 0.000 4.244 *Fit Size/Strain: XS(Å) = 33 (1), Strain(%) = 0.805 (0.0343), ESD of Fit = 0.00902, LC = 0.751

57
Center for Materials Science and Engineering http://prism.mit.edu/xray Analysis Mode: Fit Size Only slope= 0= strain FW(S)*Cos(Theta) Sin(Theta) 0.0000.784 0.000 4.244 *Fit Size Only: XS(Å) = 26 (1), Strain(%) = 0.0, ESD of Fit = 0.00788, LC = 0.751

58
Center for Materials Science and Engineering http://prism.mit.edu/xray Analysis Mode: Fit Strain Only y-intercept= 0 size= ∞ FW(S)*Cos(Theta) Sin(Theta) 0.0000.784 0.000 4.244 *Fit Strain Only: XS(Å) = 0, Strain(%) = 3.556 (0.0112), ESD of Fit = 0.03018, LC = 0.751

59
Center for Materials Science and Engineering http://prism.mit.edu/xray Analysis Mode: Fit Size/Strain Pos. [°2Th.]FWHM Left [°2Th.] Integral Breadth [°2Th.] Crystallite Size only [Å] Micro Strain only [%] Shape Left 40.2733(5)0.829(1)1.30279377.1754301.4496521.000(3) 58.282(2)1.188(5)1.50625469.7112101.1345750.50(1) 73.221(2)1.371(4)2.15426153.5427901.2061821.000(7) 87.053(5)1.67(1)2.51461550.5653801.1059960.91(2) 100.729(5)2.18(2)3.40623842.5669901.1748990.99(2)

60
Center for Materials Science and Engineering http://prism.mit.edu/xray Comparing Results Size (A)Strain (%)ESD of Fit Size(A)Strain(%)ESD of Fit Size Only 22(1)-0.011125(1)0.0082 Strain Only -4.03(1)0.03513.56(1)0.0301 Size & Strain 28(1)0.935(35)0.012532(1)0.799(35)0.0092 Avg from Scherrer Analysis 22.525.1 Integral BreadthFWHM

61
Center for Materials Science and Engineering A large amount of crystallite size or microstrain will hinder analysis of the other term Both microstrain and crystallite size can be analyzed only when the broadening due to both is equivalent When the amount of microstrain is large, the maximum observable crystallite size will be limited –A 1% microstrain might limit the maximum crystallite size to as little as 40 nm. The small amount of broadening due to a larger crystallite size will not be accuratey quantified When the crystallite size is small, the maximum quantifiable microstrain will be limited http://prism.mit.edu/xray

62
Center for Materials Science and Engineering http://prism.mit.edu/xray Other Ways of XRD Analysis Most alternative XRD crystallite size analyses use the Fourier transform of the diffraction pattern Variance Method –Warren Averbach analysis- Fourier transform of raw data –Convolution Profile Fitting Method- Fourier transform of Voigt profile function Whole Pattern Fitting in Fourier Space –Whole Powder Pattern Modeling- Matteo Leoni and Paolo Scardi –Directly model all of the contributions to the diffraction pattern –each peak is synthesized in reciprocal space from it Fourier transform for any broadening source, the corresponding Fourier transform can be calculated Fundamental Parameters Profile Fitting –combine with profile fitting, variance, or whole pattern fitting techniques –instead of deconvoluting empirically determined instrumental profile, use fundamental parameters to calculate instrumental and specimen profiles

63
Center for Materials Science and Engineering http://prism.mit.edu/xray Complementary Analyses TEM –precise information about a small volume of sample –can discern crystallite shape as well as size PDF (Pair Distribution Function) Analysis of X-Ray Scattering Small Angle X-ray Scattering (SAXS) Raman AFM Particle Size Analysis –while particles may easily be larger than your crystallites, we know that the crystallites will never be larger than your particles

64
Center for Materials Science and Engineering http://prism.mit.edu/xray Textbook References HP Klug and LE Alexander, X-Ray Diffraction Procedures for Polycrystalline and Amorphous Materials, 2 nd edition, John Wiley & Sons, 1974. –Chapter 9: Crystallite Size and Lattice Strains from Line Broadening BE Warren, X-Ray Diffraction, Addison-Wesley, 1969 –reprinted in 1990 by Dover Publications –Chapter 13: Diffraction by Imperfect Crystals DL Bish and JE Post (eds), Reviews in Mineralogy vol 20: Modern Powder Diffraction, Mineralogical Society of America, 1989. –Chapter 6: Diffraction by Small and Disordered Crystals, by RC Reynolds, Jr. –Chapter 8: Profile Fitting of Powder Diffraction Patterns, by SA Howard and KD Preston A. Guinier, X-Ray Diffraction in Crystals, Imperfect Crystals, and Amorphous Bodies, Dunod, 1956. –reprinted in 1994 by Dover Publications

65
Center for Materials Science and Engineering http://prism.mit.edu/xray Articles D. Balzar, N. Audebrand, M. Daymond, A. Fitch, A. Hewat, J.I. Langford, A. Le Bail, D. Louër, O. Masson, C.N. McCowan, N.C. Popa, P.W. Stephens, B. Toby, “Size- Strain Line-Broadening Analysis of the Ceria Round-Robin Sample”, Journal of Applied Crystallography 37 (2004) 911-924 S Enzo, G Fagherazzi, A Benedetti, S Polizzi, –“A Profile-Fitting Procedure for Analysis of Broadened X-ray Diffraction Peaks: I. Methodology,” J. Appl. Cryst. (1988) 21, 536-542. –“A Profile-Fitting Procedure for Analysis of Broadened X-ray Diffraction Peaks. II. Application and Discussion of the Methodology” J. Appl. Cryst. (1988) 21, 543-549 B Marinkovic, R de Avillez, A Saavedra, FCR Assunção, “A Comparison between the Warren-Averbach Method and Alternate Methods for X-Ray Diffraction Microstructure Analysis of Polycrystalline Specimens”, Materials Research 4 (2) 71-76, 2001. D Lou, N Audebrand, “Profile Fitting and Diffraction Line-Broadening Analysis,” Advances in X-ray Diffraction 41, 1997. A Leineweber, EJ Mittemeijer, “Anisotropic microstrain broadening due to compositional inhomogeneities and its parametrisation”, Z. Kristallogr. Suppl. 23 (2006) 117-122 BR York, “New X-ray Diffraction Line Profile Function Based on Crystallite Size and Strain Distributions Determined from Mean Field Theory and Statistical Mechanics”, Advances in X-ray Diffraction 41, 1997.

66
Center for Materials Science and Engineering http://prism.mit.edu/xray Instrumental Profile Derived from different mounting of LaB 6 In analysis of Y 2 O 3 on a ZBH, using the instrumental profile from thin SRM gives a size of 60 nm; using the thick SRM gives a size of 64 nm

Similar presentations

© 2017 SlidePlayer.com Inc.

All rights reserved.

Ads by Google